Advanced Computational Materials Science: Application to Fusion and Generation IV Fission Reactors
Fusion and Generation IV
U. S. Department of Energy
Office of Science
Office of Nuclear Energy, Science, and Technology
Workshop on Advanced Computational Materials Science:
Application to Fusion and Generation IV Fission Reactors
U.S. Department of Energy
Office of Science
Office of Nuclear Energy, Science, and Technology
31 March – 2 April 2004
Dr. Raymond L. Orbach
Director, DOE Office of Science
Dr. William D. Magwood, IV
Director, DOE Office of Nuclear Energy, Science, and Technology
on behalf of the workshop participants by the organizers:
Roger E. Stoller, Metals and Ceramics Division
Steven J. Zinkle, Metals and Ceramics Division
Jeffrey A. Nichols, Computer Science and Mathematics Division
William R. Corwin, Metals and Ceramics Division
Oak Ridge National Laboratory
30 June 2004
Table of Contents
Executive Summary 3
1. Session I: Overview of Relevant Irradiation Environments 8
2. Session II: Current State of the Art in Relevant Multiscale Computational Materials
Science Models 16
3. Session III: Goals and Targets for Understanding and Predicting Material Performance 27
4. Session IV: Expected Advances and Contributions of Computational Science 41
Summary and Recommendations 54
Appendix A Workshop Agenda 58
Appendix B Workshop Participants 65
Appendix C Acronyms and Abbreviations 67
The ORNL research staff who were responsible for organizing the Workshop and assembling
this report gratefully acknowledge the contributions of all the workshop participants to the success of
the meeting, and to the technical and editorial content of the report. In particular, those members of the
International Advisory Committee who served as session chairmen, Drs. Patrick Ledermann, David
Bacon, Nasr Ghoniem, and David Keyes, acted as lead authors for the chapters developed from their
The Workshop on Advanced Computational Materials Science: Application to Fusion and
Generation IV Fission Reactors was convened to determine the degree to which an increased effort in
modeling and simulation could help bridge the gap between the data that is needed to support the
implementation of these advanced nuclear technologies and the data that can be obtained in available
The need to develop materials capable of performing in the severe operating environments
expected in fusion and fission (Generation IV) reactors represents a significant challenge in materials
science. There is a range of potential Gen-IV fission reactor design concepts and each concept has its
own unique demands. Improved economic performance is a major goal of the Gen-IV designs. As a
result, most designs call for significantly higher operating temperatures than the current generation of
LWRs to obtain higher thermal efficiency. In many cases, the desired operating temperatures rule out
the use of the structural alloys employed today. The very high operating temperature (up to 1000˚C)
associated with the NGNP is a prime example of an attractive new system that will require the
development of new structural materials. Fusion power plants represent an even greater challenge to
structural materials development and application. The operating temperatures, neutron exposure levels
and thermo-mechanical stresses are comparable to or greater than those for proposed Gen-IV fission
reactors. In addition, the transmutation products created in the structural materials by the high energy
neutrons produced in the DT plasma can profoundly influence the microstructural evolution and
mechanical behavior of these materials.
Although the workshop addressed issues relevant to both Gen-IV and fusion reactor materials,
much of the discussion focused on fusion; the same focus is reflected in this report. Most of the physical
models and computational methods presented during the workshop apply equally to both types of
nuclear energy systems. The primary factor that differentiates the materials development path for the
two systems is that nearly prototypical irradiation environments for Gen-IV materials can be found or
built in existing fission reactors. This is not the case for fusion. The only fusion-relevant, 14 MeV
neutron sources ever built (such as the rotating target neutron sources, RTNS-I and -II at LLNL) were
relatively low-power accelerator based systems. The RTNS-II “high” flux irradiation volume was quite
small, less than 1 cm3, and only low doses could be achieved. The maximum dose data obtained was
much less than 0.1 dpa. Thus, RTNS-II, which last operated in 1986, provided only a limited
opportunity for fundamental investigations of the effects of 14 MeV neutrons characteristic of DT
Historically, both the fusion and fission reactor programs have taken advantage of and built on
research carried out by the other program. This leveraging can be expected to continue over the next ten
years as both experimental and modeling activities in support of the Gen-IV program grow
substantially. The Gen-IV research will augment the fusion studies (and vice versa) in areas where
similar materials and exposure conditions are of interest. However, in addition to the concerns that are
common to both fusion and advanced fission reactor programs, designers of a future DT fusion reactor
have the unique problem of anticipating the effects of the 14 MeV neutron source term. In particular, the
question arises whether irradiation data obtained in a near-prototypic irradiation environment such as
the IFMIF are needed to verify results obtained from computational materials research. The need for a
theory and modeling effort to work hand-in-hand with a complementary experimental program for the
purpose of model development and verification, and for validation of model predictions was extensively
discussed at the workshop. There was a clear consensus that an IFMIF-like irradiation facility is likely
to be required to contribute to this research. However, the question of whether IFMIF itself is needed
was explored from two different points of view at the workshop. These complementary (and in some
cases opposing) points of view can be coarsely characterized as “scientific” and “engineering.”
The recent and anticipated progress in computational materials science presented at the
workshop provides some confidence that many of the scientific questions whose answers will underpin
the successful use of structural materials in a DT fusion reactor can be addressed in a reasonable time
frame if sufficient resources are devoted to this effort. For example, advances in computing hardware
and software should permit improved (and in some cases the first) descriptions of relevant properties in
alloys based on ab initio calculations. Such calculations could provide the basis for realistic interatomic
potentials for alloys, including alloy-He potentials, that can be applied in classical molecular dynamics
simulations. These potentials must have a more detailed description of many-body interactions than
accounted for in the current generation which are generally based on a simple embedding function. In
addition, the potentials used under fusion reactor conditions (very high PKA energies) should account
for the effects of local electronic excitation and electronic energy loss. The computational cost of using
more complex potentials also requires the next generation of massively parallel computers. New results
of ab initio and atomistic calculations can be coupled with ongoing advances in kinetic and phase field
models to dramatically improve predictions of the non-equilibrium, radiation-induced evolution in
alloys with unstable microstructures. This includes phase stability and the effects of helium on each
However, for all its promise, computational materials science is still a house under construction.
As such, the current reach of the science is limited. Theory and modeling can be used to develop
understanding of known critical physical phenomena, and computer experiments can, and have been
used to, identify new phenomena and mechanisms, and to aid in alloy design. However, it is
questionable whether the science will be sufficiently mature in the foreseeable future to provide a
rigorous scientific basis for predicting critical materials’ properties, or for extrapolating well beyond the
available validation database.
Two other issues remain even if the scientific questions appear to have been adequately
answered. These are licensing and capital investment. Even a high degree of scientific confidence that a
given alloy will perform as needed in a particular Gen-IV or fusion environment is not necessarily
transferable to the reactor licensing or capital market regimes. The philosophy, codes, and standards
employed for reactor licensing are properly conservative with respect to design data requirements.
Experience with the U.S. Nuclear Regulatory Commission suggests that only modeling results that are
strongly supported by relevant, prototypical data will have an impact on the licensing process. In a
similar way, it is expected that investment on the scale required to build a fusion power plant (several
billion dollars) could only be obtained if a very high level of confidence existed that the plant would
operate long and safely enough to return the investment.
These latter two concerns appear to dictate that an experimental facility capable of generating a
sufficient, if limited, body of design data under essentially prototypic conditions (i.e. with ~14 MeV
neutrons) will ultimately be required for the commercialization of fusion power. An aggressive theory
and modeling effort will reduce the time and experimental investment required to develop the advanced
materials that can perform in a DT fusion reactor environment. For example, the quantity of design data
may be reduced to that required to confirm model predictions for key materials at critical exposure
conditions. This will include some data at a substantial fraction of the anticipated end-of-life dose,
which raises the issue of when such an experimental facility is required. Long lead times for
construction of complex facilities, coupled with several years irradiation to reach the highest doses,
imply that the decision to build any fusion-relevant irradiation facility must be made on the order of 10
years before the design data is needed.
Two related areas of research can be used as reference points for the expressed need to obtain
experimental validation of model predictions. Among the lessons learned from ASCI, the importance of
code validation and verification was emphasized at the workshop. Despite an extensive investment in
theory and modeling of the relevant physics, the NIF is being built at LLNL to verify the performance
of the physics codes. Similarly, while the U.S. and international fusion community has invested
considerable resources in simulating the behavior of magnetically-confined plasmas, a series of
experimental devices (e.g. DIII-D, TFTR, JET, NSTX, and NCSX) have been, or will be, built and
numerous experiments carried out to validate the predicted plasma performance on the route to ITER
and a demonstration fusion power reactor
A renewed interest in nuclear reactor technology has developed in recent years, in part as a
result of international interest in sources of energy that do not produce CO2 as a by-product. One result
of this interest was the establishment of the Generation IV International Forum (http://gen-
iv.ne.doe.gov/ ), which is a group of international governmental entities whose goal is facilitating
bilateral and multilateral cooperation related to the development of new nuclear energy systems. At the
same time, advances in plasma physics and fusion engineering have raised interest in the feasibility of
fusion energy employing the deuterium-tritium (DT) fusion reaction. This is evidenced by the
international effort to build the ITER (http://www.ofes.fusion.doe.gov/iter.html) as the first fusion
science experiment capable of producing a self-sustaining fusion reaction. ITER is seen as the essential
next step on the path of demonstrating the scientific and technological feasibility of fusion energy.
Interest in fusion is sufficiently high that international panels have recommended a “fast track” approach
to developing fusion energy source, shown for example in reports at:
http://fire.pppl.gov/eu_fast_track_101201.pdf and http://www.naka.jaeri.go.jp/ITER/ITER-
Because of the significant challenges associated with structural materials applications in these
advanced nuclear energy systems, the Workshop on Advanced Computational Materials Science:
Application to Fusion and Generation IV Fission Reactors was convened by the U.S. Department of
Energy’s Office of Science and the Office of Nuclear Energy, Science and Technology to ensure that
research funded by these programs takes full advantage of ongoing advancements in computational
science and the Department’s investment in computational facilities. In particular, participants in the
workshop were asked to:
(1) Examine the role of high-end computing in the prediction of materials behavior under the
full spectrum of radiation, temperature, and mechanical loading conditions anticipated for
advanced structural materials that are required for future Generation IV fission and fusion
reactor environments, and
(2) Evaluate the potential for experimentally-validated computational modeling and
simulation to bridge the gap between data that that is needed to support the design of
these advanced nuclear technologies and both the available database and data that can be
reasonably obtained in currently-available irradiation facilities.
An international panel of expert materials and computational scientists was invited to participate
in the workshop. The workshop program is provided in Appendix A and the final makeup of the panel is
listed in Appendix B. In addition to the panel, a number of interested scientists attended as observers
and were given the opportunity to contribute to the workshop discussion. The list of observers is also
included in Appendix B.
The workshop discussion focused on metals and alloys that will be used in the regions with the
greatest potential for radiation-induced effects to occur, i.e. materials close to the fission reactor core or
the fusion plasma. This limited scope does not imply that these are the only materials issues that need to
be addressed for the successful implementation of Gen-IV or fusion reactors. Ceramics and ceramic
composite materials and graphite will be used in the highest temperature, and some high neutron flux,
regions of fission reactors such as the NGNP. Ceramics and composites will also see service in fusion
reactors, both as structural components and as insulators in regions where radiation will lead to property
degradation. In addition to the need for structural alloys, a number of other special purpose materials
such as tungsten, copper, or SiC may see service in high heat flux, plasma-facing components. In some
cases, the radiation damage issues for these materials are similar to those addressed in the workshop, but
others also arise. These include radiation-induced conductivity and changes in dielectric properties for
insulators, and sputtering for plasma-facing components. Thus, the workshop’s focus on structural
materials in relatively high neutron flux regions should be seen as an expedient, necessary evil due to
the limited time available.
Structural materials proposed for use in conceptual designs for Gen-IV and fusion reactors
include variants of complex ferritic-martensitic steels, superalloys, vanadium alloys, carbon-carbon
composites and silicon carbide composites. Potential coolants include helium, water, sodium, lithium
and lithium compounds, lead alloys, and molten salts. The primary method currently envisioned to
provide high strength and fracture toughness as well as appropriate radiation resistance in high-
temperature metallic components involves incorporating a high density of nanoscale second phase
features to serve as point defect recombination centers and for helium trapping. However, these
nanoscale features are intrinsically unstable under irradiation due to ballistic dissolution and other non-
equilibrium processes, such as radiation induced solute segregation and radiation enhanced diffusion.
Thus, a key challenge is to design materials for which the duration of the transient non-equilibrium
stage is greatly increased. For this approach to be successful, the metastable nanoscale features must be
maintained to damage levels approaching 200 displacements per atom (dpa). Understanding the stability
of these features requires development of models that couple dissolution, segregation, and diffusion in
complex systems. While the basis for components of such a complex model exist, the ability to integrate
modeling components is still lacking.
The unique aspects of the DT fusion reactor environment, and the differences from fission
reactors, predominantly arise from the differences between the DT and fission neutron energy spectra.
Fission neutrons are born with a broad spectrum of energies peaking near 0.65 MeV (the flux at 10 MeV
is reduced by a factor of 350), whereas the DT fusion neutron spectrum is essentially mono-energetic at
14.1 MeV. Although the energy of the fusion neutrons is quickly reduced by collisions with the
materials that comprise the reactor structure, materials nearest the plasma are exposed to a neutron
energy spectrum that is significantly different from that obtained in fission reactors. The effect of these
higher energy neutrons is two-fold. First, fusion neutrons will obviously produce higher energy
displacement cascades than the lower-energy fission neutrons. Based on coordinated modeling and
experimental studies performed over the past 15 years, it appears the defects produced by fission and
fusion cascades will be qualitatively similar and that displacement cascade damage differences can be
accounted for using the well-established dpa unit of exposure.
The second effect of higher energy neutrons in the fusion spectrum is enhanced nuclear
transmutation reactions , due to the existence of nuclear reactions with threshold energies between 2
and 15 MeV in many structural materials. The production of solid transmutants (particularly surface-
active impurities) can alter alloy properties. The transmutation products of greatest concern are
hydrogen and helium because these gases can significantly impact microstructural evolution and be
synergistic with displacement damage phenomena. Although a variety of theoretical and experimental
techniques have been applied to examine the role of helium on microstructural stability and mechanical
property changes, key aspects of the behavior and effects of helium remain unresolved. As a simple
example, helium is known to stabilize small radiation-induced vacancy clusters. Depending on the ratio
of helium to displacement production, this stabilization can lead to either more or less void swelling
[2,3], and a significant reduction in creep rupture times and ductility due to enhanced grain boundary
1. K. Ehrlich, Phil. Trans. R.. Soc. London A 357 (1999) 595.
2. V. Levy, D. Gilbon and C. Rivera, in Effects of Radiation in Materials, 12th International
Symposium, ASTM STP 870, F. A. Garner and J. S. Perrin, Eds., ASTM International, West
Conshohocken, PA, 1985, p. 317.
3. R. E. Stoller and G. R. Odette, in Effects of Radiation in Materials, 11th International Symposium,
ASTM STP 782, H. R. Brager and J. S. Perrin, Eds., ASTM International, West Conshohocken, PA,
1982, p. 275.
1. Session I: Overview of Relevant Irradiation Environments
1.1 Objectives of Session I
This opening session was intended to provide a description of the operating environments for
structural materials applications in anticipated advanced fission (Generation IV) and DT fusion reactors.
The goal was to highlight the similarities and differences among the various exposure conditions for the
purpose of informing the discussion in the following sessions. Potentially useful experimental facilities
such as test reactors and ion irradiation facilities were also discussed, as was the possible relevance of
spallation neutron sources which provide a similar challenge to materials performance .
1.2 Introduction to Irradiation Environments
Generation IV and DT fusion systems are expected to supply energy in a sustainable manner to
modern economies for centuries. In this context, the word energy primarily implies electrical generation
and the delivery of process heat at high temperatures for purposes such as hydrogen production. In order
to obtain the desired dramatic advances in performance over current fission systems, advanced fission
and fusion systems will operate in regimes and environments that are beyond current nuclear industry
experience, as well as most previous experience with developmental fission systems [2, 3]. Materials
must perform at higher temperatures and for longer times, and to larger irradiation doses than required
in current light water reactor technology. In additional, some advanced nuclear system designs propose
coolants that are more aggressive than high-temperature water. For successful deployment of advanced
fission and fusion systems, significant advances in material technology are required.
In many important ways, the materials for fusion and fission systems face similar temperature,
radiation, and corrosion environments. Table 1-1 below provides a general comparison of the range of
operating conditions expected in advanced nuclear systems. Even among concepts with different
coolants, many application requirements have important similarities (such as temperature, stress, or
neutron spectrum), prompting selection of similar materials, or classes of materials.
Table 1-1. Advanced fission and fusion operating conditions
Fusion Fission (Gen-IV)
Coolant H2O, He, Li, PbLi, FLiBe H2O(SC), He, Pb, PbBi, Na
Particle Energy < 14 MeV < 1–2 MeV
Temperatures 300-1000˚C 300–1000˚C
Max displacement damage ~ 200 15–200
He/dpa 10 appm/dpa ~ 0.1 appm/dpa
Stresses Moderate, nearly constant Moderate, nearly constant
The materials of construction must demonstrate adequate mechanical strength, ductility, and
toughness, must demonstrate adequate dimensional stability, must maintain adequate thermo-physical
properties, and must have acceptable resistance to corrosion and stress corrosion attack from cooling
media . Experimental programs cannot cover the breadth of materials and irradiation conditions for
the proposed fusion and Gen-IV fission reactor designs. A set of tools is required to assist in a material
selection process that will be performed based on an incomplete experimental database and that requires
considerable judgment to carry out the necessary interpolation and extrapolation. Modeling and
microstructural analysis can provide the intellectual foundation for these important decisions.
Materials degradation from radiation starts with collisions between high-energy neutrons and
lattice atoms and then develops into radiation-induced microstructures that degrade mechanical
properties, dimensional stability, thermo-physical properties, and resistance to environmental attack.
This is true in both fission and fusion systems. A set of computational tools that adequately describes
radiation events and subsequent microstructural development and provides from this microstructure an
accurate description of property changes in engineering materials would be a tremendously valuable
tool for system designers. While developing these computational tools into a truly predictive capability
is a difficult and time-consuming challenge, the knowledge gained from development of the individual
model components will provide valuable insight to any on-going materials design effort. These models
cannot be developed without a parallel set of validation experiments. The interplay between new
experimental data and advanced theory or computational tools is critical to the development of accurate
radiation response models.
While there are many similarities between fission and fusion systems, some important
differences do exist. For example, the higher energy neutrons in fusion systems will lead to greater
concentrations of the transmutation gasses helium and hydrogen. Additionally, certain Gen-IV concepts
use different coolants and may respond to changes in microstructure in a unique manner. These
differences do not dramatically change the types of computational tools that need to be developed. The
tools need to encompass broad time and length scales from descriptions of primary damage formation
all the way to bulk property changes. Properly done, this basic set of tools will be valid for both fission
and fusion. The differences in environment will dictate only that a broader set of confirmatory
experiments is required to ensure the models are valid over the entire operating regime of fission and
1.3 Related Research and Development Issues
In addition to a survey of the relevant irradiation environments, the members of this group also
discussed the issue of materials needs for advanced nuclear energy systems from three different
perspectives. Here their overview encompassed:
• Irradiation environments and the physical and chemical processes engendered by
• Computational capabilities required
• Research and development and engineering objectives
The first perspective concentrated on the physical and chemical processes involved in radiation
damage and in changes to relevant materials properties, and the second reviewed computational
methods and how they map onto the physical and chemical processes that must be modeled and
evaluated computationally. Finally, the desired outcomes were enumerated and an assessment was made
of the nature and extent of information required to enable design of new reactor concepts without
construction of many prototypes or extensive testing.
1.3.1 Irradiation Environments and the Physical Processes Engendered by Radiation Damage
The progress achieved during the last two decades in our fundamental understanding of
radiation damage in solids has shown that there exists a unified theoretical description for the majority
of the processes involved, and that these processes are essentially the same for most irradiation
environments. It then follows that a complete theoretical formulation of all the processes and all the
cause-effect relationships must be applicable to irradiation with neutrons, electrons, γ-rays, ions, and
fission products. Conversely, results obtained from a particular irradiation environment must be useful
Radiation source: n, e-, γ, fission products and ions
Atomic Displacement Cascades and Electronic Excitation
Primary damage: PKA, Point Defects, He, H, Irradiation Environment: T,
solid transmutation products Stress, Radicals
In-cascade Clustering Diffusion
Defect Cluster Formation and Evolution Radiation Induced Segregation
Dislocation Loops and Voids Bubbles Precipitate
Co-evolution of all Microstructural
Mechanical and Dimensional Fracture, Fatigue, Corrosion and
Thermo-physical Changes and Creep Stress Rupture Compatibility
Figure 1-1. Schematic diagram of radiation damage processes
for all others. In the past, the complexity of radiation damage processes required simplified treatments
tailored to a specific radiation environment, and the models so obtained were limited. Today, and even
more so in the near future, advanced computational materials science can take full advantage of the
universal theoretical description of radiation damage. Naturally, many of the processes need to be dealt
with, be refined and validated, but the entire edifice can now be clearly recognized in its overall shape
and scope. Figure 1-1 presents a rather compact rendition of this edifice. It shows that the radiation
sources all produce primary recoil atoms via elastic collisions  that in turn produce collision cascades
[6, 7], the sources for defects and defect clusters .
At the elevated temperatures existing in nuclear reactors, these defects diffuse, dissolve, and re-
aggregate in other forms throughout the material. These secondary defects evolve into a complex new
microstructure, and in the process, change microscopic and macroscopic properties of the material. This
picture holds for both metallic alloys and insulators. In addition, inelastic collisions are known to affect
the chemical bonds of insulators, creating charged defects which will also diffuse and induce changes in
related macroscopic properties.
1.3.2 Computational Capabilities Required
Many of the theoretical tools required have already or are being developed by a much larger
group of experts active in many branches of solid-state physics and materials science. This will greatly
benefit the smaller group of scientists active in the area of radiation damage. The tools can be grouped
in four main classes that include different types of models as shown in the flow chart in Figure 1-2,
along with their main output physical quantities.
Ab Initio Calculations
Interatomic Potentials Fundamental properties of defects, defect
clusters, and interactions between defect
Primary defect production
MD Simulations Diffusion of defects and their reactions
Dislocation motion (glide/climb)
Kinetic MC Microstructure and
Methods precipitate evolution
DD, Mesoscopic and Plastic properties and
Continuum Methods Fracture
Correlation of radiation effects data from neutron, electron, and ion irradiations
Extrapolations to higher doses and lower dose rates
Figure 1-2. Summary of computational tools and their uses in radiation damage modeling
These models have typically been developed and applied to pure elements or simple dilute
alloys. In contrast, the high in-service temperature and radiation levels typical of nuclear application
require multi-element concentrated alloys with optimized chemical compositions and microstructures.
The reliability of the prediction of multiscale modeling for nuclear materials will thus depend very
much on the capability of the nuclear materials community to select, develop, and apply models that
accurately treat the critical components of microstructural evolution in complex alloys and relate that
microstructural evolution to specific changes in macroscopic properties. An in depth analysis of the
present capabilities of these modeling tools and their future development are given in Sessions II-V.
1.3.3 Research and Development and Engineering Objectives
The computational tools must provide the basis for: (a) re-assessing existing data, (b)
optimizing new experiments in test reactors or in a dedicated neutron source (14 MeV), and (c)
interpreting the obtained data and reliably extrapolating them to anticipated in–service conditions, the
domain of which is always broader than those achieved in experiments. The ultimate goal is to use the
experimentally validated models to enable scientists to improve existing materials or to design better
For engineering purposes, the computed and measured property changes need to be codified
into databases or constitutive relationships that an engineer can use to design a nuclear energy system,
assess its performance, and determine its ultimate lifetime.
1.4 Near-term Research Priorities
Although there is a vast number of physical changes induced by irradiation, some phenomena
are either already understood at a sufficient (albeit rudimentary) level for evaluating feasibility issues, or
are not critical determining factors in establishing the feasibility of using materials in irradiation
environments. Conversely, there are several fundamental radiation effects phenomena that critically
need improved understanding in order to assess candidate material options. These include defect
production and evolution in alloys and ceramics (as opposed to pure metals), coupled solute-defect
diffusion processes in concentrated alloys, microstructural evolution of coupled point defect sinks (e.g.,
voids and dislocations), and the effects of point defect clusters, surface active transmutant impurities
and helium on localized deformation and fracture toughness. These are briefly discussed in the
A firm understanding of the fundamentals of defect production and evolution in alloys is
essential for evaluating the microstructural stability of candidate engineering materials in
experimentally unexplored irradiation conditions. The current defect production modeling efforts have
been largely limited to pure metals such as Fe and Cu. It is well known from fundamental experiments
performed with ion and fission neutron irradiation sources that the production and evolution
(annihilation, clustering) of point defects and defect clusters is significantly different in alloys compared
to pure metals. This appears to be due to enhancement or suppression of point defect recombination
within the displacement cascade as well as solute effects on point defect mobility and trapping at solute
precipitates. Subtle differences in minor alloying elements in complex engineering alloys have been
observed to have a pronounced effect on their stability during neutron irradiation. As a first step toward
accurate modeling of prospective engineering alloys, suitable interatomic potentials need to be derived
for important binary alloy and ternary systems including Fe-Cr, Fe-Ni, Fe-He, and Fe-Cr-Ni. To
properly account for the behavior of steels, the influence of C and N also need to be included. An
improved understanding of helium effects in irradiated materials is of particular importance for fusion
energy, since recent simulation experiments suggest that fusion-relevant helium generation during
neutron irradiation may have severe deleterious effects on the dimensional stability and fracture
toughness of current candidate alloys. Similar improvements in the fundamental understanding of defect
production and evolution in irradiated nonmetals such as ceramic insulators are also needed. In
particular, the conditions for production of defects in nonmetals by pure ionizing radiation (radiolysis
and high electronic stopping power processes) need to be accurately understood so these effects can be
separated from knock-on collision effects. The migration and annihilation processes of charged and
uncharged point defects in nonmetals also need to be understood.
There is a strong need to develop improved physically based models and simulations of
radiation-induced and -enhanced segregation processes. The current segregation models used by many
researchers are based on models originally developed in the 1970s (solute drag and inverse Kirkendall
effects). Dramatic improvement was achieved in the 1990s by the introduction of models that used
atomistic information to account for diffusion in concentrated alloys . However, many of the key
physical parameters in these models are not well known, including the binding energies and migration
energies of various solute-point defect complexes as a function of the local composition. On a broader
level, the kinetics and mechanisms of diffusion in concentrated alloys in the presence of solute gradients
are not sufficiently known. This opens the possibility that new solute-defect coupled diffusion processes
may occur under irradiation that are not covered by the rudimentary solute drag and inverse Kirkendall
models. As a first step toward development of improved point defect-solute models, the vacancy
formation energy and migration energy should be determined as a function of solute content (including
carbon) in iron and other important material systems. The role of dumbbell interstitials, particularly
mixed solute-solvent dumbbells, also requires further investigation.
Current models of radiation-induced void swelling treat voids and network dislocations as
separately evolving systems that are linked only by the effect of void and dislocation sink strengths on
the arriving point defect fluxes. However, experimental studies have found that dislocations thread
voids in many cases. Therefore, it may not be appropriate to model void and dislocation evolution
during irradiation as weakly interacting systems. Kinetic Monte Carlo studies of microstructural
evolution in the presence of coupled point defect sinks (voids/dislocations) would be valuable to provide
guidance on the importance of this coupling. The effect of helium generation on this coupling could be
subsequently investigated. The effect of chemical segregation on the development of microstructural
features should also be studied.
The advent of 3-dimensional dislocation dynamics during the past decade has been a major
achievement for modeling numerous important materials phenomena. However, dislocation climb
processes have not yet been modeled in 3-dimensional dislocation dynamics codes. Inclusion of the
various modes of dislocation climb would enable 3-dimensional dislocation dynamics to be
quantitatively applied to investigations of microstructural evolution of irradiated materials. A further
challenge is how to develop the appropriate linkages of 3-dimensional dislocation dynamics to atomic
scale and mesoscale regimes so that multiscale phenomena such as fracture toughness can be
There are numerous deformation and fracture phenomena that need improved understanding.
For example, there is current debate within the research community whether the long-standing
connection between cleared dislocation channels and low tensile elongations is a bona fide cause and
effect in metals irradiated at low temperatures. Improved multiscale models are needed to analyze
potential causes of the low ductility in irradiated metals and to identify possible metallurgical solutions
to mitigate this effect. The effects of point defect clusters and helium bubbles on crack formation and
propagation also need to be investigated. It is uncertain whether there are any new He-enhanced fracture
toughness degradation mechanisms at low temperatures beyond normal matrix hardening effects.
Development of physically realistic multiscale models, combined with experimental studies, could
provide important insight in this critically important area. Similarly, the potential effect on deformation
and fracture of surface-active impurities produced by neutron transmutation reactions should be
investigated. There is a largely incomplete understanding of the physical phenomena responsible for the
poor elevated temperature ductility of superalloys during irradiation. If the physical processes
responsible for the low ductility of superalloys irradiated at high temperatures could be identified and
mitigated, superalloys would be attractive candidates for fission Gen-IV and fusion systems. Finally,
despite nearly 40 years of research, a comprehensive model for high temperature helium embrittlement
is not yet in place. High temperature helium embrittlement is anticipated to limit the maximum
allowable doses and temperatures for structural alloys in fusion and Gen-IV fission reactors, and
appropriate multiscale models and experiments should provide guidance for metallurgical improvements
to increase the dose and temperature limits.
1.5 Validation and Verification of Models
Validation and verification of the predictions made by computational models can be performed
using either established benchmarked computational codes or experimental data. Computational
benchmarking and validation/verification of model predictions can also be obtained by comparing the
results obtained from several different computer codes or techniques applied to analyze a similar
scenario. Direct validation and verification of model predictions can be obtained in many cases by
performing appropriate experiments. The experimental data for model validation and verification can be
grouped into five categories:
(1) Mining of old data: Previously published experimental data represents an important
resource that should be fully utilized in order to minimize costs associated with
mounting new experiments. Experimental studies on fundamental point defect or
materials properties are of particularly high value. Appropriate caution must be applied
in extracting experimental data from published studies, since most data have been
processed using models of varying degrees of robustness. In some cases, previously
reported experimental data may need correction to account for deficiencies in the
models originally used to analyze the test results.
(2) Mining of old reactor materials: Archive irradiated specimens from prior nuclear
energy programs should be preserved wherever feasible for future experimental study.
Due to rising costs for storage and disposition of radioactive materials, there is
increasing pressure to dispose of specimens that are not of immediate value. These
specimen storage costs must be weighed against the costs and technical value of
performing new specifically designed experiments to obtain the same data. Of course,
in many cases new experiments may provide opportunities to obtain data of
significantly improved quality.
(3) Irradiation experiments using ion implantation, electrons, fission neutrons and
spallation neutrons should be designed and performed to elucidate or quantify specific
mechanisms that are building blocks in the multiscale modeling framework. These
mechanistic experiments span the range from single-variable tests to multiple-variable
synergistic phenomena studies. In many cases, specifically designed experimental
techniques (such as tritium doping or He injector foils for studying He effects) may
provide important insight on the controlling physical mechanisms.
(4) Prototypic irradiation experiments enable the opportunity to systematically investigate
single-variable or synergistic multiple-variable effects on material coupons under
environmental conditions similar to the intended application (e.g., DT fusion neutron
spectrum or supercritical water irradiation assisted stress corrosion cracking
phenomena). These prototypic tests are traditionally of very high value for confirming
the predictions of computational models and establishing the safety basis for gaining
licensing approval of reactors.
(5) Component testing: Integral irradiation experiments on reactor components (such as
fusion reactor blanket modules) should eventually be tested in a dedicated facility.
Integral tests of this kind are essential to validate that all the detailed models of
materials performance are integrated in a seamless manner, and more importantly, that
synergistic effects and phenomena are captured and well understood before a new
reactor is built. Component testing is generally not initiated until the separate-effects
data obtained from coupon testing in prototypic environments are fully analyzed using
In addition to providing predictive insight on potential physical mechanisms, computational
models can provide important hindsight by explaining archive experimental results. Appropriate
computational models are essential for obtaining maximum usefulness of data obtained in nonprototypic
Several categories of experimental data are needed for computational model validation and for
licensing. The most fundamental information is associated with point defect and defect cluster
properties (formation, migration and binding energies, relaxation volume, 1-D vs. 3-D diffusion
characteristics, etc.). These fundamental properties generally cannot be obtained directly from
experiment, but instead are inferred from experimental observations by utilizing appropriate models.
There are numerous classic examples in the literature where published fundamental data have required
subsequent correction due to neglect of important physical phenomena in the original data analysis.
Important experimental tools for acquiring fundamental radiation effects data on point defects and
defect clusters include a variety of X-ray diffraction techniques, electrical resistivity methods, stored
energy, positron annihilation spectroscopy, density, high resolution and microanalytical transmission
electron microscopy, Mössbauer spectroscopy, optical spectroscopy, elastic moduli tests, and a variety
of mechanical property measurements. The microstructural evolution of irradiated materials involves
integration of multiple phenomena over extended time periods and length scales. Experimental
observations obtained from electron microscopy, X-ray diffraction, positron annihilation, and other
microstructural tools are valuable for validating and calibrating multiscale computational models. The
microstructural evolution drives a number of important changes in physical and mechanical properties
that can be used in concert with microstructural investigations to experimentally verify and validate
multiscale model predictions. Important mechanical properties for engineering purposes include tensile
elongation, tensile strength, thermal and irradiation creep, fracture toughness, fatigue strength, and
fatigue crack growth rate.
4. L. K. Mansur, A. F. Rowcliffe, R. R. Nanstad, S. J. Zinkle, W.. R. Corwin, and R. E. Stoller,
“Materials Needs for Fusion, Generation IV Fission Reactors, and Spallation Neutron Sources -
Similarities and Differences, 11th International Conference on Fusion Reactor Materials, Kyoto,
Japan, December 2003, to be published in J. Nucl. Mater.
5. A Technology Roadmap for Generation IV Nuclear Energy Systems, Report No. GIF002-00,
December 1, 2002 (http://nuclear.gov).
6. E. E. Bloom, S. J. Zinkle, and F. W. Wiffen, “Materials to Deliver the Promise of Fusion Power,”
11th International Conference on Fusion Reactor Materials, Kyoto, Japan, December 2003, to be
published in J. Nucl. Mater.
7. Higher Temperature Reactor Materials Workshop, ANL-02/12, Argonne National Laboratory,
8. L. R. Greenwood, J. Nucl. Mater. 216 (1994) 29.
9. R. S. Averback, J. Nucl. Mater. 216, (1994) 49.
10. R. E. Stoller and L. R. Greenwood, J. Nucl. Mater. 271&272 (1999), 57.
11. L. K. Mansur, J. Nucl. Mater. 216 (1994) 97.
12. M. Nastar, Defect and Diffusion Forum 194-199 (2001) 171.
2. Session II: Current State of the Art in Relevant Multiscale Computational Materials
2.1 Objectives of Session II
The subpanel responsible for Session II was charged with characterizing the adequacy of the
current state-of-the-art in multiscale computational materials science models for the purpose of
simulating radiation effects in structural materials. The participants determined that it will be necessary
to set in place over the next five-to-ten year period a suite of computational tools to model, predict and
guide assessment of ferritic steels under relevant conditions of damage, helium generation, temperature,
time and stress. The crucial properties for simulations of reactor materials radiation damage are (a)
defect creation; (b) defect migration and interaction; (c) boundary structure and segregation effects; (d)
dislocation behavior under stress; and (e) phase stability. It is essential that the modeling techniques be
robust and versatile enough to treat other materials and other problems that enter the frame over the time
period. Furthermore, the tools must be able to guide future experiments as well as be informed by them.
This section devotes considerable attention to atomic-scale methods because radiation damage
in reactor components is created at this scale and the evolution of damage is controlled by processes on
this scale. Furthermore, recent advances in such computationally-based methods offer exciting
opportunities for prediction of materials properties in situations where experimental information is
unavailable. Nevertheless, the scope for computational materials science to tackle important problems at
the continuum scale must not be lost sight of: yielding, creep and fracture are examples of processes
where simulation is required across all scales. In terms of increasing length and time scales, the relevant
modeling aspects considered include ab initio methods, interatomic potentials, molecular dynamics and
other methods of treating materials discretely at the nano-to-micro scale, continuum-based modeling
and developments for simultaneous linking of length and time scales. Current developments are
discussed in the following sections, but first we consider some of the current issues involved.
2.2 Overview of Current Issues
Molecular dynamics (MD) is the most widely used method for atomic-scale simulation. Much
of our current understanding of, for example, primary damage in cascades, point defects and their
clusters, dislocation core properties and crack-tip processes, comes from MD simulation. In MD, the
classical equations of motion are integrated to obtain dynamical evolution of a system of atoms.
Accurate integration requires time steps in the femtosecond range, limiting the total simulation time to
less than a microsecond on today's processors. Direct MD is a powerful probe, giving the classically
exact dynamical evolution of a system for a given interatomic potential. It provides for determination
and prediction of material properties at the atomic scale and, since higher-level models for materials
evolution (kinetic Monte Carlo (KMC), dislocation dynamics, phase field models, rate theory, etc.)
involve assumptions and approximations about properties, it offers a benchmark for their verification.
Advances in interatomic potentials described below in section 2.3 will mean that MD simulations can be
compared directly to experiment. Two possible exceptions to this are light atom (hydrogen or helium)
diffusion below room temperature, where quantum corrections to the dynamics start to become
important, and dynamics during the thermal spike stage of a cascade, when non-Born-Oppenheimer
effects omitted from MD become important (e.g., thermal transport via electron-phonon coupling in a
metallic system or electronic excitations in a covalently bonded system).
Computer memory sets the upper limit for the number of particles, i.e. the system length scale.
Fortunately, the static or dynamic properties of relatively small subsystems often determine the
macroscopic materials behavior. This explains the widespread use and success in materials science of
electronic band structure calculations, molecular statics and MD simulations. However, MD parallelizes
well via spatial decomposition, offering an easy path to extend the length scale. Simulations of a million
atoms are routine, billion-atom simulations have been performed, and it should be possible to simulate
~1011 atoms (= one-micron cube of Fe) for approximately a microsecond on the next-generation
leadership-class machine. Increasing model size will allow unprecedented direct examination of
phenomena, such as multi-dislocation interactions and fracture. This means, for instance, that
displacement cascades created by primary recoils with energy up to a few 100keV can be simulated,
although electronic effects (excitation and electron-phonon coupling) are likely to remain difficult to
incorporate in MD models. Since subcascade formation is common in most metals at the higher energies
in this range, the use of Binary Collision Approximation (BCA) codes, tuned to MD results at
overlapping energy, is expected to be fruitful.
Time scales accessible to MD are more problematic. The calculation of the energy and
interatomic force is by far the most expensive part of an MD simulation, so complexity in the
interatomic potentials should be avoided. Model size is currently limited to about a thousand atoms if
accurate quantum mechanically derived forces are used and larger systems mentioned in the preceding
paragraph have to be described by more approximate force fields. Total simulation time and/or model
size is expected to continue to increase proportionally to single-processor speed, but physical limitations
in processor design will cause this to flatten out in the next 5-10 years. Consequently, direct MD
simulations of million-atom systems may never reach one millisecond, even with simple potentials. As
many important activated phenomena (diffusion, defect clustering, void growth, grain growth,
dislocation motion, creep, etc.) are active on time scales orders of magnitude beyond this, this poses a
critical problem. Thus, methods of speeding up MD simulation are required. We address this in section
2.4. These techniques are not applicable to many classes of problem, however, and then it is necessary
to use either the MC or continuum methods described below.
The nature of dislocation motion within the microstructure of an irradiated material is a major
factor to be considered for assessing the in-service integrity of reactor components. Motion can occur as
a result of either applied stress, internal stress or chemical stress due to point defects, and gives rise to
phenomena as varied as uniform flow, localized yielding, hardening, crack tip plasticity and creep. Until
recently, most models of dislocation glide and climb in the presence of defects created by damage fluxes
were based on the elasticity theory of dislocations, with line shape under stress estimated using the line
tension approximation. This approximation neglects the effects of self-interaction between different
parts of the line, which, for dislocations overcoming obstacles, can have an important influence on the
flow stress. A dislocation with self-stress can be modeled as a flexible line constructed of piecewise
segments. Although self-stress was first treated in this way over 30 years ago , it was only possible to
consider a few hundred segments for a few tens of iterations. Ideally, 3D dislocation dynamics (DD)
models of plasticity on the micro-meso scale require the simulation of 0.1-100mm of line length (for a
dislocation density of 1014m-2), and thus contain typically 105-108 segments. They should also be able to
achieve a total plastic strain at realistic strain rates (e.g. 10% at 10-6s-1). These aims cannot be met at the
moment. Hence, new, more efficient techniques for computing the field of segments and their
interactions with each other and damage microstructure are required. As discussed in section 2.5, these,
coupled with expected advances in computing power, will enable the goals to be met.
Continuum-based DD models have uncertainties associated with singularities in the dislocation
stress field and the loss of validity of the elasticity description at the atomic scale. These limitations do
not apply to MD simulation of dislocation behavior. Hence, MD modeling can provide detailed
information on obstacle forces  and dislocation core effects  for incorporation in larger scale DD
simulation. However, the requirements on MD for treatment of plasticity at the length and time scales of
interest are many orders of magnitude beyond current computing power. For example, limits on
simulated time restrict the modeling of dislocation glide to strain rates of about 106 per second, whereas
rates a billion times smaller are of primary concern. For dislocation-controlled creep, the rates of
interest are orders of magnitude smaller again. Thus, the limitations and benefits of using this method
have to be recognized. Current work is discussed in section 2.5.
It is necessary to ensure that the atomic system is not dominated by artificial boundary effects,
i.e. it should behave as a representative part of the surrounding macrosystem. For instance, band
structure theory utilizes periodic boundary conditions to mimic an infinite solid. In more general
situations, defects break translational symmetry and more complicated boundary conditions are needed.
This problem is closely related to the length scale limitations. Except for the case of free clusters,
boundary effects such as stress or strain, temperature or heat flux have to be applied to the atomistic
system. In addition, energetic events, e.g. interaction of high-energy atomic particles with solids, create
pressure waves, which, without careful choice of boundary conditions, can cause inaccuracies in the
evolution of the subsystem.
Simultaneous coupling of different methods with appropriate spatial resolution and accuracy
can overcome such problems and also raise the limits of atomistic system size. The multiple length
scales are covered by continuum mechanics (for the macroscopic part of the material), computationally
inexpensive interatomic potentials (bridging the mesoscale where the atomic motion has to be resolved)
and quantum-derived forces (for high accuracy in the nanoscale parts where strong non-equilibrium
processes prevail). Radiation damage and crack formation are examples where hybrid schemes can be
valuable, i.e. accurate forces are required close to a strong local disturbance, its neighborhood can
exhibit thermal or mechanical disorder for which simple empirical forces are adequate, and the long-
range response can be supplied by a surrounding continuum. The general issue of coupling across the
scales is considered further in section 2.5.
The evolution of microstructure and properties of materials under intense energy input may be
controlled by essentially kinetic phenomena and so not understood in thermodynamic terms only. The
main methods used currently to predict the kinetics are, in order of increasing space and time scales, the
various forms of KMC (mostly on Rigid Lattice, Event-based or Object-based), Self-consistent Mean
Field, Phase Field, and Cluster Dynamics (Rate Theory) models. In order to develop robust, physically-
based models for predicting the kinetic pathways and “dynamic phase diagrams,” it is necessary to
calculate accurately the populations and elementary properties of point defects, and determine the
detailed mechanisms of atomic migration on which the evolution models are based. Recent
developments of first principles methods, coupled with fast computation techniques to explore
configurations in systems of increasing size, allows complex defects and alloys to be considered [4,5].
The coupling of first principles calculation with kinetic models is now being validated with success
against experimental data, thereby demonstrating the robustness of this approach. It is described further
in section 2.7.
2.3 Interatomic Potentials
2.3.1 Current status
MD and MC simulations require an interatomic potential that represents the energy and forces
associated with a configuration of atoms in a real material. To be usable for complex geometries and/or
statistical averages, the potential needs to be computed rapidly. Many interatomic potentials have been
developed and are reported in the literature, but none are necessarily adequate for simulation of the wide
range of properties required for reactor materials. With pair-wise interactions some are necessarily
wrong. With many-body potentials (used here as a generic term covering glue, Finnis-Sinclair,
embedded atom, modified embedded atom and effective medium theory potentials) many can be fitted
provided “correct” values are available. These types of potentials have been the “state of the art” for
Historically, there has been an insufficient database for robust potential fitting. Not all this data
is available experimentally for parameterization and verification of potentials. Recent renewed interest
in interatomic potentials is based on the ability of ab initio calculations to provide this missing data –
with teraflop machines verification of predictions is finally possible. Where tested against new data,
existing potentials have generally proved disappointing. Problems include incorrect self-interstitial
configuration and energy, and no satisfactory description of the austenitic-ferritic transition. Some
problems can be traced to parameterization of the potentials and addressed by simple
reparameterization. Others, such as the absence of a physically sensible treatment of magnetization,
point to more fundamental problems in the many-body potential concept.
Most effort for metallic phases has focused on elemental materials. Potentials for some multi-
component systems have been developed, but their predictive capability is typically disappointing.
Reasonable models for the mission-critical helium impurities exist, the inertness of helium making its
behavior in MD somewhat insensitive to parameterization. There are two challenges in the development
of potentials for alloy systems. First, there is generally much less data available, though this can be
rectified through the use of ab initio methods. Second, the appropriate functional forms are not as well
developed. Most potentials are based on simple pictures of bonding. In alloy systems, the nature of the
bonding is inherently more complex, suggesting that more sophisticated potentials are needed. Non-
metallic impurities, such as carbon and phosphorus, are more problematic.
The advent of ab initio calculations has allowed more accurate verification procedures to be
applied to existing models, and highlighted some serious flaws. The prospects for rectifying these are
good: some are simply a matter of reparameterization and extension to systems where insufficient
underpinning data existed previously [6,7]; others require implementation of new models already
proposed ; some may require the development of new approaches. The primary resource requirement
for these developments is manpower, inspiration and stronger interactions between research groups to
understand one another’s needs.
2.3.2 Where do we need to go with interatomic potentials?
Discussions at the workshop highlighted three areas regarding interatomic potentials that
warrant attention for further development.
18.104.22.168 Validation and reparameterization of existing many-body models.
The technology for validation based on ab initio simulation is mature. A database of structures
and migration paths for point defects with and without impurities needs to be created. (This will also
benefit calculation at the KMC level). Efficient fitting techniques based on genetic algorithms can be
employed to assist parameterization. Crucial data not available currently ab initio includes defect
migration mechanisms, dislocations core states and defect-dislocation interactions, and will require
22.214.171.124 Development of better models for magnetism and alloying.
It is possible to create potentials with more complex functional forms than currently, but with
similar computational complexity. Two new types have been proposed in Europe and should be
exploited by the program.
The two-band model represents the electronic structure on each atom by a single, local,
variational parameter µ. This has been applied to describe the volume-collapse transition in Cs where
µrepresents s-d transfer . The model has potential applicability to ferritic steels where µ is the
magnetization, and to materials where f-localization is important. The functional complexity does not
result in additional computational complexity thanks to the Hellmann-Feynman theorem, which means
that the force can be evaluated without differentiating µ.
Composition-dependent potentials offer the possibility to incorporate non-local Fermi-surface
effects by making the potential dependent on the global as well as local electron density. This addresses
such anomalies as the multiple bcc-fcc-hcp phase transitions observed with many short-range potentials
under pressure. Here the functional form throughout the simulation is modified according to the
composition and density of the MD simulation cell. This is practical since almost all MD simulations
conserve particle number. There are some problems with constant pressure MD, since a fictitious term
appears in the pressure – however since all applications of constant pressure MD already have a
fictitious mass in the Lagrangian this issue should be tractable with perturbative corrections akin to the
Pulay stresses encountered in plane-wave DFT. Simple composition-dependent potentials have been
applied to dilute Fe-Cr alloys which exhibit an oscillatory alloying energy that cannot be reproduced
with conventional many-body potentials.
These two models, and a reawakened interest in new model complexity, offer tremendous
promise for extending existing MD models to the complex multi-component steels and to properly
understanding the atomic basis of the role of minority additives in determining bulk properties. This in
turn opens the possibility of guiding development of materials, reducing the number of samples required
to be synthesized for experimental testing.
126.96.36.199 Interaction with applied mathematics community
The underlying challenge is to develop a computationally convenient representation of the
energy and forces between atoms that can be computed from ab initio methods. This can be viewed as
an applied mathematics problem of finding a reliable representation of a known complex function. A
clear opportunity exists for collaborations between the physics and mathematics communities to develop
novel approaches to the challenge of representing the Born-Oppenheimer surface for a variety of
2.4 Molecular Dynamics: Accelerated Molecular Dynamics Methods
It seems clear that many of the important phenomena in irradiated materials will have to be
studied over the next few years by classical MD with computationally-simple interatomic potentials, i.e.
millions of atoms for times on the order of a nanosecond, or thousands of atoms for perhaps a
microsecond. However, in the last few years, a new class of methods  aimed at the micro-to-milli-
second time scale has emerged. Their goal is to propagate the system rapidly from state to state in a
correct fashion without introducing assumptions or prior knowledge about the possible mechanisms for
diffusion or reaction. This is a departure from the KMC approach, for in accelerated MD methods the
system finds its own way out of each state without prior specification of the mechanisms. Applying
statistical mechanical concepts, this escape process is stimulated to occur more quickly, but with little,
or no, corruption of the probabilities for escape along any given path. In this way, a volume of material
can be evolved forward from state to state out to much longer times than are possible with standard MD.
In the temperature accelerated dynamics method (TAD) , with a few controlled approximations the
computational speedup (‘boost factor’) can reach into millions  when the barriers are high relative to
the temperature, i.e. TAD can reach time scales of seconds and beyond on a single processor. This has
been demonstrated for vapor-deposited film growth of copper  and radiation annealing of low-energy
cascades in MgO . For systems with persistent low barriers, which are common for realistic cases,
however, the boost factor is more modest and improving on this limitation (without introducing
significant approximations) is an important area of ongoing research. In the parallel-replica dynamics
(PRD) method  time is parallelized. PRD is very general, requiring only that the reactive processes
be first-order (exhibit exponential first-passage statistics), and that transitions can be detected. An
appealing feature of PRD is that it gives exact state-to-state dynamics, with parallel speedup, if properly
implemented. There is no assumption of Arrhenius behavior, nor even that there is an energy barrier
associated with reactive events, i.e. the bottleneck can be purely entropic. Inter-processor
communication requirements are minimal; parallel efficiency can be maintained up to the point where
the time between reactive events has been collapsed to the order of the correlation time (a few ps for a
transition metal system). Thus, for events separated by a few microseconds, a computational boost
factor on the order of a million could be achieved on a million processors. However, as noted above, the
more typical case is that low barriers in the system limit this boost.
Besides this boost limitation, the other key remaining issue for these methods is the accessible
length scale. The TAD method in its present form becomes inefficient for systems larger than ~1000
atoms due to the fact that the computational work scales super-linearly with system size. For the PRD
method, the system size matters only in that for larger systems there tend to be more available activated
processes, with decreasing average time between events and maximum possible parallel boost. The low-
barrier and length scale issues are the subject of ongoing research, and should be considered for future
These new methods offer opportunities for unprecedented investigations on the next generation
of massively parallel computers. One example would be parallelizing both for electronic structure, and
then, multiplicatively, for PRD. If the electronic structure-based MD could reach, say, 200 ps, then
parallel-replica dynamics could follow the system through about 40 transitions. This could allow the
first view of post-cascade dynamics on the microsecond time scale with full electronic structure
2.5 Dislocation Dynamics
2.5.1 3D dislocation dynamics
Dislocation Dynamics (DD) simulations approach is becoming an increasingly important tool in
the computational materials research [13, 14]. Over the last several years there have been considerable
advances both in the general DD methodology and in its implementation on massively parallel
computers. The uniqueness of DD is its ability, on one hand, to incorporate the atomistic mechanisms of
dislocation motion and interactions (among dislocations and with other elements of material
microstructure) and, on the other hand, to directly compute the plastic strength of crystalline materials.
Thus, DD provides a much-needed bridge between the length and time scales of the fundamental
physical mechanisms and the length and time scales relevant for engineering applications.
Three major challenges for further development of the DD approach are that (1) the unit
mechanisms of dislocation motion and interaction are multiple and complex, (2) one needs to trace the
evolution of very large groups of dislocations over extended periods of time while accessing the length
and time scales relevant for microstructure evolution and its effects on yield, flow, strain hardening and
strain localization, and (3) development of connections between DD and continuum plasticity theory.
Recent achievements of 4-10% of plastic strain in a direct DD simulation suggest that the approach is on
its way to becoming computationally efficient, through the use of massively parallel computing and
more advanced numerical algorithms. The most serious of the remaining computability challenges is to
scale DD simulations down to lower straining rates (~10-5) and yet maintain their computational
efficiency. The problem here is to be able to handle multiple time scales observed in the evolution of
large dislocation populations, where periods of relative calm (slow motion of lines) are interspersed
with bursts of very high activity over which small groups of lines moves very fast and experience
Parallel DD implementations face their own problems. The first one is a programming
challenge: the DD models deal with the ever-changing topology of dislocation lines and line networks
requiring rather complex data structures and careful bookkeeping. On parallel machines, this challenge
is dramatically amplified due to the need to handle the network topology across the boundaries of
computational domains. The second challenge is a natural tendency of dislocation lines to cluster in
space (owing to the long-range interactions among the lines) and develop highly heterogeneous
distributions of degrees of freedom making it difficult to achieve a good load balance. The code
ParaDiS recently written at LLNL has shown much promise in addressing these challenges .
DD simulations of radiation-damaged materials share the challenges of fidelity and
computability and add some more. As an example, the need to account for explicit dislocation-
SFT/loop/cluster interactions places even higher demands on the computational throughput of the DD
codes. Still more complex and computationally challenging will be to describe, within a single model,
the concurrent evolution of dislocation-, alloy- and radiation defect-microstructures which is a key issue
for predictive modeling of fission and fusion reactor materials. Several attempts have been made to
couple KMC lattice simulations of the radiation defect microstructure with the DD simulations. While
possible in principle, such coupling makes both DD and KMC simulations still more expensive than
they are in isolation. At the same time, the phase field models that have been successfully used in the
past for modeling alloy microstructure evolution were recently advanced to model dislocations and their
motion. However, the phase-field DD models cannot compete with the line-tracking DD when it comes
to combining high resolution with computational efficiency. As a possible way to reduce the
computational complexity while achieving a degree of coupling between dislocation and defect sub-
systems, it appears possible and in fact desirable to combine the line-tracking DD method (to handle the
dislocation sub-structure) with a mesh-based phase-field approach (to handle the alloy field evolution).
2.5.2 Atomic-level simulation of dislocations
Computer modeling of dislocation processes relevant to damage microstructures can readily
simulate several millions of atoms. With suitably designed periodic boundary conditions, dislocation
glide over distances many tens of nm can be studied, and interaction with obstacles of realistic spacing
can be treated. The importance of understanding dislocation-obstacle interaction at the atomic level was
demonstrated by Rodney and Martin  for the glide of an edge dislocation through an interstitial
dislocation loop in Ni. The absorption of the loop and jog formation, leading to pinning effects on the
dislocation, was shown in detail. Since then, simulations of dislocation interactions with SFTs, loops,
voids and precipitates have been reported, e.g. [2,17,18], including the screw dislocation . With
suitable boundary conditions for application of force or displacement, it is possible to extract
quantitative information on the relationships between applied stress, strain rate, temperature, obstacle
size and spacing for a given material [2,18]. However, with limited MD timescales (~ns), plastic strain
rates of at least 106s-1 are unavoidable. Thus, results on, say, applied stress and/or dislocation
configuration have to be tested against changes in strain rate and temperature in order to assess their
possible applicability to much longer timescales.
As an alternative to MD, molecular statics (MS) may be employed to mimic the equilibrium
state at 0K by minimizing the potential energy of the system. With many atoms and complex reactions,
it is not always possible to guarantee that a true minimum is achieved, and processes that depend on
temperature may be missed. Nevertheless, by increasing the applied strain incrementally, equilibrium
line and obstacle configuration under increasing stress can be found, e.g. [2,18]. This approach has the
advantage that the results should be directly comparable with those given by models based on elasticity
theory for the equilibrium of dislocations under stress. In fact, MS simulation of strengthening due to
voids and precipitates in Fe [2,18] show that the earlier continuum treatments of these obstacles [2,20]
have wider applicability than expected. The next challenge is to extract the effective obstacle shear
resistance stress from the MS and/or MD simulations and incorporate them in DD simulations, thereby
achieving nano-scale accuracy in micro-scale modeling.
2.6 Coupling Schemes
2.6.1 Empirical force field ↔ continuum (MM/CM)
The way different zones exchange information is crucial for the performance of a hybrid
scheme. Several schemes have been suggested for the coupling between atoms in the empirical force
field zone and the nodes of the numerically discretized continuum [21-24]. Ideally one would like to
meet two requirements: (i) energy conservation and (ii) bias-free forces in the boundary area. However,
a critical review of currently available methods  clearly reveals that one cannot achieve both. The
schemes of [21,22] fulfill criterion (i) but require additional ghost forces to keep the boundary atoms on
their lattice sites. The other schemes [5,22] neglect the concept of a global Hamilton function with the
benefit of an exact representation of boundary atom forces. Since the motion of nodes is conceptually
not intended to represent the thermal energy of the continuum, one might think that requirement (i) is
less important. Additional complications occur when short wave length disturbances cross the zone
Differences in the high frequency part of the phonon dispersion laws of the different zones
cause backscattering of the short-wavelength part of the transmitted elastic wave. This artifact can by
avoided by applying a low-pass filter at the boundary absorbing the high-frequency components .
2.6.2 Quantum force field ↔ empirical force field (QM/MM)
In addition to the exchange of atomic displacement information at the zone boundary, the
electrons in the quantum zone require electronic information from the MM region (which is at first not
available). According to Kohn’s principle of near sightedness  only the electrons in a small
boundary layer of the MM region influence the solution of the Schrödinger equation in the QM zone.
Depending on the material, the problem to obtain electronic information in the MM zone can be solved
in different ways. Ionic systems represent the simplest material class, since only the Madelung potential
from the MM region influences the QM solution. For covalent systems an artificial hydrogen saturation
of the bonds crossing the QM/MM boundary can be performed . An alternative Green’s function
(G) approach assumes the presence of the lattice G outside the QM region  as a QM boundary
condition. For metallic systems, a bond order expansion of the electronic density of states leads to a real
space method  requiring only atomic information from the MM medium.
2.6.3 Learn on the fly
The so called learn on the fly method (LOF) represents an alternative to the traditional QM/MM
coupling . The whole QM/MM region is described by a suitable empirical force field with spatially
varying parameters. The force field is locally reparameterized (using a corresponding quantum force
calculation for a localized cluster of atoms) if strong deviations from equilibrium configurations occur
during the dynamical evolution of the system.
2.6.4 Related questions and future development
The most important question is the relevance of simultaneous-multiscale schemes for fusion and
Gen-IV fission related materials. The MD description of radiation damage and related component
failure represents an important cornerstone on the way to an understanding and design of the required
strong materials. In the past, simulations were focused on a qualitative understanding of the relevant
processes and it was sufficient to employ simple empirical potentials for a very limited class of
materials (Lennard-Jones Ar and embedded atom Cu are typical examples) and using very simple
boundary conditions (fixed atoms, periodic boundary conditions, analytic asymptotic continuum
solutions). This clearly marks the childhood of computational materials science. In order to enter
maturity more elaborate models with quantitative predictive power are required. Alloys are by far more
complicated than pure copper and therefore the accuracy of the interatomic forces is a pressing problem.
For localized disturbances, QM/MM or LOF schemes might provide valuable tools to achieve high
precision where it is needed. The success of these methods will also depend on the development and
improvement of linear scaling electronic structure methods which will allow accurate treatment of ten
thousands of atoms in the near future. For a quantitative description of even larger non-equilibrium
systems, empirical potentials with near quantum precision are mandatory and development into this
direction also needs a strong support. Empirical bond order alloy potentials are a significant step in this
In order to be really predictive, one must not neglect the exact influence of macroscopic
boundary conditions on the outcome of the microscopic dynamics in high energy collision cascades,
thermal spikes and crack motion. For crack propagation  or energetic particle surface collisions 
it is already a standard procedure to embed the atomistic region into a continuum. For radiation damage
of MeV cascades, it has to be applied in the near future .
Up to now the continuum is treated with the discretized differential equations of elasticity
theory. Other continuum descriptions using mesoparticle dynamics  would allow for crack
propagation from the microscopic zone into the embedding medium. The development into this
direction is very interesting and could result in a powerful alternative to span the length scales.
2.7 Multiscale Modeling of Thermodynamics and Kinetics under Irradiation
A first step in the modeling of microstructure evolution is to predict the thermodynamic
properties of complex systems, not always available experimentally. In addition to first principles
calculations of cohesive energies, from which formation enthalpies  are deduced, very powerful
numerical calorimetry methods based on Static MC methods have been developed which give access to
the thermodynamic functions of complex systems where the configuration entropy cannot be calculated
explicitly . This is the case of amorphous or strongly distorted crystalline structures.
The Rigid Lattice KMC methods are extremely efficient for studying the incubation and
nucleation of precipitates, and can now be validated with experiments at the same scale as the modeling
box (10-5 µm3) using the 3D Atom Probe, a technique which has recently achieved close to atomic
resolution. They are used to identify the complex sequence of metastable and stable precipitation (or
“dynamic phase diagrams”) in alloys, to control materials strength and brittleness by influencing
nucleation and coarsening, notably by identifying additives to enhance nucleation and hinder
coarsening. They are particularly well adapted to test and integrate refined energetic and diffusion
models, e.g. . Recently, they have been upgraded to tackle irradiation effects by implementing all
the interstitial diffusion mechanisms, PD sources and sinks, thus allowing for point defects fluxes
towards sinks which are responsible for Radiation-Induced Segregation and Precipitation (RIS & RIP).
As they give access to the details of evolution at the atomic scale for all the atoms in the calculation
box, these techniques are demanding in CPU time (roughly proportional to the number of jumps
performed) and therefore limited to relatively small time and space scales, which in turn depend on
temperature and atomic binding energies that control the jump probabilities. Also, they require
knowledge of elementary parameters (binding and saddle point energies), which must be very accurate
in view of the high sensitivity of kinetics to some of these parameters, whose number, in addition,
becomes quite large in even moderately complex alloys. The massive input of first principles data is
A limitation of the Rigid Lattice approach is that it does not allow for systems and phenomena
with large size effects (i.e. large elastic constraints), at least not with an accuracy equivalent to that
achieved for the effects of purely chemical bonds. For such situations, however, Relaxed Lattice MC
techniques are being developed to account for diffusion and precipitation in systems with large atomic
and/or particle size effects, notably the coherent–incoherent transition in precipitation. These
developments are promising, but are hindered by the enormous CPU time requirement .
Systems of larger dimension (µm3) and comprising complex objects can be explored with the
help of Event-Based KMC models, in which the MC algorithm is not applied to individual atomic jumps
but to the probability of impingement or dissociation of populations of mobile defects and immobile
objects . This is possible at the expense of detailed spatial localization, which is no longer at the
atomic scale. Such models are well adapted to account for recovery of complex point defects and defect
cluster populations in pure metals and dilute alloys during and after irradiation , and especially the
effect of microstructural features such as dislocations, grain boundaries, precipitates, free surfaces etc,
which of course requires that their sink and source strengths are correctly implemented.
In order to deal with concentrated, multi-component, heterogeneous systems over wider time
and space scales, Self-Consistent Mean Field diffusion models are used. They describe the diffusive and
thermodynamic properties at the same level of approximation, accounting for all the correlations
between atomic jumps, and for both the thermodynamic and kinetic coupling of fluxes. The latter is of
paramount importance for materials under irradiation as it gives rise to RIS at grain boundaries in
stainless steels , for example. Also, such models are designed to take advantage of existing
macroscopic data bases (e.g. DICTRA) and enrich them with atomic scale-based calculations.
In order to describe the overall evolution of single defect and defect cluster populations without
space or time limitation, one can resort to Rate Theory (Cluster Dynamics) in conjunction with TEM
and 3D Atom Probe experiments, e.g. to understand the formation mechanism of defects and solute
clusters responsible for the hardening and embrittlement of steels under neutron irradiation . They
have been recently extended and applied to precipitation in cubic alloys and the irradiation growth of
hexagonal metal systems.
The atomistic approach is also used to check, validate and improve mesoscopic kinetic models,
namely nucleation, growth and coarsening theory. This formalism is based on a few basic quantities,
essentially the nucleation driving force and the interface free energy, which are not accurately known
but can be calculated on a safe physical basis using first principles methods, atomic scale models of
interactions and diffusion, and statistical mechanics techniques (e.g. precipitation in complex alloys
1. D.J. Bacon, U.F. Kocks and R.O. Scattergood, Phil. Mag. 28 (1973) 1241.
2. Yu.N. Osetsky and D.J. Bacon, Model. Simul. Mater. Sci. Eng. 11 (2003) 247.
3. J. Marian, W. Cai and V. Bulatov, Nature Materials 3 (2004) 158.
4. C.C. Fu, F. Willaime and P. Ordejon, Phys. Rev. Let. 92 (2004) 175503.
5. M. Fähnle Defect and Diffusion Forum 194-199 (2001) 279.
6. M.I. Mendelev, S. Han, D.J. Srolovitz and G.J. Ackland, Phil. Mag. 83 (2003) 3977.
7. G.J. Ackland M.I. Mendelev, D.J. Srolovitz, S. Han and A.V. Barashev, J. Phys. C, in press (2004).
8. G.J. Ackland and S.K. Reed, Phys. Rev. B 67 (2003) 174108.
9. A.F. Voter, F. Montalenti and T.C. Germann, Annual Rev. Mater. Res. 32 (2002) 321.
10. M.R. Sorensen and A.F. Voter, J. Chem. Phys. 112 (2000) 9599.
11. B.P. Uberuaga et al, Phys. Rev. Let. 92 (2004) 115505.
12. A.F. Voter, Phys. Rev. B 57 (1998) 13985.
13. H. M. Zbib, V. Bulatov and T. Diaz de la Rubia, Trans. ASME 74 (2002) 78.
14. N. M. Ghoniem, S.-H. Tong, and L. Z. Sun, Phys. Rev. B 139 (2000) 913-927.
15. V. Bulatov, W. Cai, J. Fier, M. Hiratani, T. Pierce, M. Tang, M. Rhee, K. Yates and T. Arsenlis,
Supercomputing 2004, submitted.
16. D. Rodney and G. Martin, Phys. Rev. B 61 (2000) 8714.
17. J.S. Robach, I.M. Robertson, B.D. Wirth and A. Arsenlis, Philos Mag. 83 (2003) 995.
18. Yu. N. Osetsky, D. J. Bacon and V. Mohles, Phil. Mag. 83 (2003) 3623.
19. D. Rodney, Acta Mater. 52 (2004) 607.
20. R.O. Scattergood and D.J. Bacon, Acta Metall. 20 (1982) 1665.
21. S. Kohlhoff, P. Gumbsch and H.F. Fischmeister, Phil. Mag. A 6 (1991) 851.
22. E.B. Tadmor, M. Ortiz, and R. Phillips, Phil. Mag. A 73 (1996) 1529.
23. M. Moseler, J. Nordiek and H. Haberland, Phys. Rev. B 56, (1997) 15439.
24. J. Q. Broughton, F. F. Abraham, N. Bernstein, and E. Kaxiras, Phys. Rev. B 60 (1999) 2391.
25. W.A. Curtin and R.E. Miller, Model. Simul. Mater. Sci. Eng. 11 (2003) 33.
26. W. Kohn, Phys. Rev. Let. 76 (1996) 3168.
27. F.F. Abraham, J.Q. Broughton, N. Bernstein and E. Kaxiras, Europhys. Let. 44 (1998) 783.
28. N. Bernstein, Europhys. Let. 55 (2001) 52.
29. A.P. Horsfield, A.M. Bratkovsky, D.G. Pettifor and M. Aoki, Phys. Rev. B 53 (1996) 1656.
30. A. de Vita and R. Car, Materials Research Society Symposium Proceedings 491 (1998) 473.
31. K. Albe, K. Nordlund and R.S. Averback, Phys. Rev. B 65 (2002) 195124.
32. J. Riedle, P. Gumbsch and H.F. Fischmeister, Phys. Rev. Let. 76 (1996) 3594.
33. M. Moseler, O. Rattunde, J. Nordiek and H. Haberland, Nucl. Instrum. and Meth. B 164 (2000) 522.
34. K. Nordlund, private communication.
35. B.L.Holian, Europhys. Let. 64 (2003) 330.
36. R. P. Gupta et al., Phil. Mag. A 80 (2000) 2393.
37. M. Athènes, Phys. Rev. E 66 (2003) 16701 and 46705.
38. F. Soisson et al., Phys. Rev. B 62 (2000) 203; 65 (2002) 094103.
39. J.L. Bocquet, Defect and Diffusion Forum 203-205 (2002) 81.
40. J. Dalla Torre, J.L. Bocquet, N.V. Doan, G. Martin and E. Adam, in Microstructural Processes in
Irradiated Materials, TMS Symposium, San Diego, March 2003.
41. C.C. Fu, J. Dalla Torre, F. Willaime, J.L. Bocquet and A. Barbu, to be published
42. M. Nastar, Defect and Diffusion Forum 194-199 (2001) 171; and in Microstructural Processes in
Irradiated Materials, TMS Symposium, San Diego, March 2003; Phil. Mag. A, in press.
43. F. Christien and A. Barbu, J. Nucl. Mater. 324 (2003) 90.
44. E. Clouet, M. Nastar and C. Sigli, Phys. Rev. B 65 (2002) 94105.
3. Session III: Goals and Targets for Understanding and Predicting Material Performance
3.1 Objectives of Session III
The primary objective of this session was to define the goals and targets required for modeling
and simulation research to develop a predictive capability for material performance under the irradiation
conditions of fusion and Gen-IV fission reactors. Two main aspects of defining these objectives became
(1) identifying the critical problems for structural materials in the irradiation environment,
and clearly describing the required development pathway, and
(2) identifying the limitations of present day computational and modeling capabilities with
respect to reaching the goals and objectives defined above, while pointing out possible
approaches that can lead to achievement of the stated goals.
3.2 Background and Primary Structural Materials Issues
Development of materials that can perform reliably for long times (~60 years) in the various
Gen-IV and fusion reactor environments is a substantial challenge. In particular, fusion structures will
place unprecedented demands on materials and complex engineering systems. The demands are driven
by time-varying thermal-mechanical loads on large heat transfer structures with complex interconnected
geometries. At the same time, structural materials will face in-service degradation of their performance
sustaining mechanical properties by suffering internal damage development, macroscopic cracking,
corrosion, and inherent dimensional instabilities [1,2]. The result will be numerous and hard to predict
failure paths in the face of demanding requirements for high reliability, long life and demonstrable
safety margins. It is critical to not only develop advanced high performance materials and models for
predicting their in-service changes, but also methods to interpret these property changes in the context
of engineering assessments of integrity limits in actual reactor structures.
Structural materials are characterized by complex, multi-constituent, multiphase, highly
defected, non-equilibrium microstructures that mediate an array of complex mechanical properties.
Properties that must be reliably modeled and predicted include:
• Yield strength and strain hardening constitutive laws.
• Various types of ‘ductility’.
• Fatigue crack growth rates.
• Fracture toughness.
• Irradiation creep rates.
• Thermal creep rates.
• Void swelling rates.
• Creep rupture times and strains.
• Thermo-mechanical fatigue stress and strain limits.
• Creep crack growth rates.
• Creep-fatigue interactions.
• Environmentally assisted cracking.
• Bulk corrosion, oxidation and compatibility.
The governing processes involve many degrees of freedom, are inherently multiscale
(time/length), and are controlled by multiple physical mechanisms that act synergistically. Critical